2 To whom all correspondences should be addressed:


 Holly Floyd
 1 years ago
 Views:
Transcription
1 Composite Modeling and Analysis of FDM Prototypes for Design and Fabrication of Functionally Graded Parts Longmei Li, Q. Sun, C. Bellehumeur 1,andP.Gu 2 Department of Mechanical and Manufacturing Engineering 1 Department of Chemical and Petroleum Engineering The University of Calgary, Calgary, Alberta, T2N 1N4, CANADA Abstract Solid Freeform Fabrication technologies have potential to manufacture parts with locally controlled properties (LCP), which would allow concurrent design of part s geometry and desired properties. To a certain extent, Fused Deposition Modelling (FDM) has the ability to fabricate parts with LCP by changing deposition density and deposition orientation. To fully exploit this potential, this paper reports a study on the mechanical properties of FDM prototypes, and related materials and fabrication process issues. Both theoretical and experimental analyses of mechanical properties of FDM parts were carried out. To establish the constitutive models, a set of equations is proposed to determine the elastic constants of FDM prototypes. An example is provided to illustrate the model with LCP using FDM. Key words: Fused Deposition Modeling, Composite Mechanics, Locally Controlled Properties. 1. Introduction With recent advances in Solid Freeform Fabrication (SFF) technologies, it is possible to use these technologies to produce parts with desired mechanical properties. The ability to fabricate parts with locally controlled properties (LCP) would create opportunities for manufacturing of a whole new class of parts with graded compositions [Jackson et al., 99] and [Cho et al., 01]. Fused Deposition Modeling(FDM) has the potential to produce parts with LCP by changing deposition density and deposition orientation. A few examples with LCP are shown in Figure 1 b), c), d), e). FDM processes fabricate prototypes by extruding a semimolten filament through a heated nozzle in a prescribed pattern onto a platform layer by layer, as in shown Figure 1 a). After the semimolten material is deposited onto the worktable it begins to cool and bond to the neighboring material diffusely. The bonding between the individual roads of the same layer and of neighboring layers is driven by the thermal energy of semimolten material. FDM processes use several types of materials, such as Acrylonitrilebutadienestyrene (ABS) and wax, to build conceptual and/or functional prototypes. Most of the existing research work in FDM is primarily directed towards the development of new materials or techniques for material deposition [Agarwala et al., 96] [Gray IV et al.,98], [Yardimci et al., 96]. The mechanical properties of ABS filament and FDM parts were also investigated by researchers such as [Comb et al., 94], [Kulkarni and Dutta, 99] and [Rodriguez Matas, 99]. ABS parts made by FDM processes essentially consist of partially bonded ABS filaments. Mechanical properties of FDM prototypes are governed by their mesostructures that are determined by manufacturing parameters. By selecting manufacturing parameters, such as deposition directions in layers and gap sizes between filaments, FDM processes can achieve LCP and produce prototypes with desired properties. To fully exploit this potential, issues concerning the mechanical properties of FDM parts and the fabrication process parameters, should be investigated. This paper describes a study on the mechanical properties of FDM prototypes. 2 To whom all correspondences should be addressed: 187
2 Figure 1: FDM process and the parts fabricated with graded mechanical properties The remaining sections of this paper consist of the following parts: Section 2 is devoted to the modeling of the mechanical properties for design of FDM parts; experimental validation is given in Section 3. Section 4 provides an example of the prototypes with graded mechanical properties using LCP. The final section summarizes the main conclusions. 2. Modeling and Analysis of Mechanical Properties of FDM Prototypes The FDM prototypes are orthotropic composites of ABS filaments, bonding between filaments and voids. They can be viewed and analyzed at different levels and on different scales. At macro level, they are studied as laminates of bonded laminars. At micro level, the properties of each laminar are functions of properties of filaments and void density. 2.1 Lamination Analysis of FDM Parts. To concurrently design mechanical geometries and properties, it is important to determine the effective stiffness so that the model can be used to predict the mechanical behaviors of the parts. Filament orientation is defined as the angle between the loading direction and longitudinal direction of filaments of each lamina. The inplane constitutive relations for the case of specially orthotropic, where = 0(or90 o ), the constitutive relation reduces to form of Equation 1: ff 11 ff22 ff = Q 11 Q12 0 Q12 Q Q ffl 11 ffl22 ffl : (1) where [ff ij ] and [ffl ij ] are the inplane stress and strain respectively. [Q] is the stiffness matrix. Four independent elastic constants, namely, longitudinal Young s modulus E11, transverse Young s modulus E22, major Poisson s ratio ν12, and shear Modulus G12 are required to describe the inplane elastic behavior of a lamina. All elements in matrix [Q] are functions of these constants. General orthotropic lamina refers to a lamina with fiber orientation other than 0 o or 90 o. Although, the stiffness matrix for general orthotropic lamina is fully populated with 6 elements. These six elements are functions of the four independent elements in matrix [Q] [Mallick, 93]. A laminate is constructed by stacking a number of laminas in the thickness direction. The 188
3 overall properties can be modeled by the Lamination Theory [Mallick, 93]. As such, in macromechanical approaches, the stiffness matrix of a laminate is composed by properties of every lamina according to the Lamination Theory, while the inplane elastic behavior of a unidirectional lamina may be fully described in terms of four elastic lamina properties including E11, E22, G12 and ν12. For the design purpose, it is desirable to have reliable predictions of lamina properties as a function of constituent properties and geometric characteristics. One of the objectives of micromechanics is to obtain such relationships. 2.2 Micromechanics of Material with Voids. A variety of methods have been used to predict properties of composite materials as functions of constituent volume ratio and geometric packing parameters. Tsai [Tsai, 64] conducted an analysis based on variational principles in which contiguity of the fibers and fiber misalignment were considered. The filament contiguity was incorporated in theoretical prediction E22, and the fiber misalignment was considered in E11. The set of the equations, when being reduced to material with voids, is depicted below. The longitudinal Young s modulus can be described by the equation: E11 = k(1 ρ1)e (2) where E is the Young s modulus of the polymer, ρ1 is the void density in Plane 1 (normal to the fibers), and k is an empirical factor that takes into account the fact that the filament may not be exactly parallel or perfectly straight. The prediction of transverse modulus, E22, takes form: E22 =(1 C) [1 (1 ρ 1)ν](1 ρ1) 1+2ρ1 ν(1 2ρ1) E (3) where ν is the Poisson s ratio of the polymer. The effective inplane shear modulus, G12, isgiven by: G12 =(1 C) 1 ρ 1 1+ρ1 G (4) where G is shear moduli of the polymer. And the inplane Poisson s ratio, ν12, isgivenbythe following relation: ν12 =(1 C)ν (5) Only the void density in the plane perpendicular to the fibers is required to compute the effective properties. The value of fiber contiguity factor C can be assigned to two extreme cases, (1) all filaments are isolated, C = 0; (2) all fibers are contiguous, C = 1. The effective Poisson s ratio, ν12, is found to be the same as that of polymer when C =0. It is the same as Hashin and Rosen s conclusion [Hashin and Rosen, 64]. Tsai s equations may be suitable for materials with cavities, but they could be used for FDM parts only under the assumption of perfect bonding among filaments. However, this assumption is not valid for the FDM process according to the ABS sintering experiments that were conducted in this research. 189
4 Figure 2: Fiber volume fraction in the transverse direction 2.3 Modeling of Elastic Constants for FDM Prototypes. The previous section demonstrated that FDM prototypes are composites of partially bonded ABS filaments and voids. Because of imperfect bonding, A new set of equations is proposed to calculate the elastic constants. When loaded in longitudinal direction, a unidirectional FDM part is an aggregate of ABS filaments. Longitudinal Young s Modulus can be predicted well by the rule of mixtures. Therefore, Longitudinal Young s Modulus is: E11 =(1 ρ1)e (6) where E is Young s Modulus of P400 filament, and ρ1 is the area void density in the plane normal to filaments. In the case of transverse normal loading, the bonding among the filaments is the load carrier. The following equation is proposed for Transverse Modulus: E22 = (1 ρ2)e (7) where is an empirical factor that takes into account the bonding strength. ρ2 is linear void fraction along the transverse direction. Refer to Figure 2, the definition of ρ2 is: ρ2 = b y : (8) b Term (1 ρ2) is the ratio of bonding length to overall dimensions. Similarly, the prediction of the inplane shear modulus takes form: G12 = (1 ρ2)g; (9) where G is the Shear Modulus of P400 filament, and the inplane Poisson s ratio, ν12, issameas that of ABS filaments, ν: ν12 = ν (10) Comparing Equations 6 through 10 with Equations 2 to 5, the significant differences are in the predictions of E22 and G12. Void density ρ2 is introduced to count the potential load carrying dimension, whereas (1 ρ1) results in the ratio of the effective load carrying media. Since the estimation of these elastic constants requires the void density in the plane perpendicular to filaments ρ1 and bond length ratio ρ2, the calculations of the void densities are the topic of the next section. 2.4 Microscopic Images Analysis. Theoretical calculations of strength, modulus, and other properties for a FDM part are based on the the void densities ρ1 and ρ2. Therefore the crosssections of FDM specimens are studied under a microscope. Unidirectional cubic specimens of dimension mm were made with different gap sizes. They were cut in the middle plane 190
5 Table 1: Results of digitized image analysis Gap Size(μm) ρ1 ρ Figure 3: Mesostructures of different gap settings. a) g = 0:100mm; b) g = 0:050mm; c) g = 0:0254mm;d) g = 0:0mm and e) g = +0:100mm which is normal to filaments. Then the photos of mesostructures were taken under a microscope, as shown in Figure 3. They were analyzed by using image processing software. Void densities ρ1 and ρ2 were calculated, and the results are listed in Table 1. From the observation and the image analysis, it can be concluded that the voids appear periodically when the negative gap is small. When the negative gap reaches 0:1mm, the dimensional accuracy and surface quality of the specimen become very poor, and the periodicity can rarely be observed. 3. Experimental Validation The theoretical stiffness model developed previously is a function of deposition densities and deposition orientations. To validate the model and method, the experimental analysis was carried out. The experiments tested the orthogonalply specimens, and the experimental results were compared with those of constitutive modeling described in Section 2. All specimens were manufactured by the FDM2000 machine. The elastic constants of P400 filaments were cited from work of Rodriguez Matas [Rodriguez Matas, 99], listed in Table 2, as the inputs of the theoretical calculations. Table 2: Elastic Properties of P400 filament Elastic Constant Value Young s Modulus, E 2230 ± 15MPa Shear Modulus, G 833 ± 7:6MPa ν 0:34 ± 0:02 191
6 E xx, N/mm Raster angle θ Figure 4: Young s modulus vs deposition Orientation in orthogonalply specimens Table 3: Orthogonalply specimen test results Specimen Young s Modulus MPa Difference Experimental Theoretical Percent [0/90] [15/75] [30/60] [45/45] The stiffness matrix of orthogonalply specimens can be constructed according to the procedure described in Section 2. As a result of the laminate modeling, the inplane Young s modulus of the orthogonalply symmetric laminates with different [ /( 90 o )] fiber orientations is a nonlinear function of the deposition angle, as shown in Figure 4. It can be observed from the figure that the laminate with raster angles of approximately [45/45] yields the minimum modulus of elasticity. The laminate with raster angles of [0/90] has the highest Young s Modulus. The experiments with the orthogonalply symmetric specimens were tested to determine the same inplane moduli. The specimens with raster angles of [0/90], [30/60], [45/45], and [15/75] were manufactured with the same thickness of 11 layers. These experimentally determined values were then compared with the theoretically predicted values to evaluate the effectiveness of the proposed laminate modeling approach, in Table 3 and marked as "Λ" in Figure 4. The experiment data were in good agreement with the results of laminate modeling. 4. Example The purpose of the study of mechanical behaviors of FDM prototypes is to establish the models for design and fabrication of the parts with the desired mechanical properties through local composition control. This can be carried out with FDM process by changing deposition density and orientations to obtain the requried properties. The design of the example part with graded mechanical properties is shown in Figure 5a). Assume that the geometrical and functional constraints require the smaller section with equal or higher stiffness than that of the larger section areas. Therefore, the properties are gradient along 192
7 Table 4: Configuration of the axis l1 l2 l3 Length(mm) Deposition strategy o [0/0] [0/90] [45/45] Gap (μm) Exx i Figure 5: An axis with gradient property. Axis X. Different deposition strategies and deposition densities were used for different sections of the part to meet the requirements as listed in Table 4. Young s modulus E xx of each section calculated according to the stiffness modeling are listed in the table. If an external axial force P is applied at each end, the overall elongation L is calculated using the following equation: 3X Z L = i=1 PL i E i xx A i(x) dx: (11) where L i is the length of each section, E i xx is the Young s Modulus of the sectoin, and A i (x) is the crosssectional area of the section. With locally controlled deposition density and deposition orientation, it is possible to make the section with smaller crosssectional area as stiff as, or even stiffer than, the section with bigger crosssectional area. 5. Concluding Remarks The design and fabrication of products with LCP would make it possible to create a new class of products with desired mechanical and material characteristics. This paper reported a study on modeling of inplane mechanical properties of FDM prototypes relating to fabrication parameters. Based on both the theoretical and the experimental analyses, a set of new equations of calculating the elastic constants were proposed and validated, which were used to determine the constitutive models of FDM parts. An example was presented to illustrate the design and fabrication of the FDM prototypes with required mechanical properties by locally controlled deposition density and orientations. Different deposition densities, angles and their combinations can be employed in producing the required stiffness properties of manufactured parts. The further study is currently underway in investigating void geometry and density with more manufacturing parameters. 193
8 Acknowledgements Thefinancial supportforthisresearch wasprovidedbythenationalsciences andengineering Research CouncilofCanada(NSERC) throughresearch GrantOGP Theauthorswould like to thank Brandon Furguson and Art Moehrle for their assistance with experiments performed intheresearch. References [Agarwala etal., 96] M. K. Agarwala, A. Bandyopadhyay, R. van Weeren, N. A. Langrana, A. Safari, and S. C. Danforth, Fused Deposition of Cerameics (FDC) for Structural Silicon Nitride Components, Solid Freeform Fabrication Symposium, Austin, TX,Aug. 8th, [Gray IVet al.,98] RobertW.GrayIV,DonaldG.BairdandJanHelgeBohn,Effectsofprocessingconditions on short TLCPfiber reinforced FDMparts, Rapid Prototyping Journal, Vol. 4, No. 1, pp , [Cho etal., 01] W.Cho, E. M. Sachs, N. M. Patrikalakis, M. Cima, T.R. Jackson, H. Liu, J. Serdy,C. C. Stratton, H. Wu, and R. Resnick, Methods for Distributed Design and Fabrication of Parts with Local Composition Control, Proceedings of the 2001 NSF Design and Manufacturing Grantees Conference, Tampa, FL,USA,January [Combet al., 94] Comb, J. W., Priedeman, W.R., and Turley, P.W.,Layered Manufacturing Control Parameters and Material Selection Criteria Manufacturing Science and Engineering, PEDVol. 682, Nov. 611, pp , [Hashin and Rosen, 64] ZviHashinandB.WalterRosen,TheElasticModuliofFiberReinforcedMaterials, Transactions of ASME:Journal ofapplied Mechanics, Vol. 86, pp , June [Jackson etal., 99] T.R. Jackson, H. Liu, N. M. Patrikalakis, E. M. Sachs, and M. J. Cima. Modeling and Designing Functionally Graded Material Components for Fabrication with Local Composition Control Materials and Design, June 1999, Vol. 20, No. 2/3, pp [Kulkarni and Dutta, 99] P.Kulkarni and D. Dutta, Deposition Strategies and Resulting Part Stiffnesses in Fused Deposition Modeling, ASME Transictions: Journal of Manufacturing Science and Engineering, Vol. 121, pp , February,1999. [Mallick, 93] P.K. Mallick, Fiberreinforced Composites: materials, manufacturing, and design, Second Edition, Marcel Dekker, Inc, [Rodriguez Matas, 99] Jose F.Rodriguez Matas, "Modeling the mechanical behavior of fused deposition acrylonitrilebutadiene styrene polymer components", Ph. DDissertation, Department of Aerospace and Mechanical Engineering, Notre Dame,Indiana, [Tsai, 64] Stephen W.Tsai, Structral Behavior of Composite Materials, NASACR71, [Yardimci et al., 96] M.Atif Yardimci, S. I.Guceri, S. C.Danforth, and M.Agarwala, "Part Quality PredictionToolsforFusedDepositionProcessing", ProceedingsoftheSolidFreeformFabricationSymposium, Austin, TX,pp , Aug
ME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationFEM Modeling of a 3D Printed Carbon Fiber Pylon
FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationComparison of Asbuilt FEA Simulations and Experimental Results for Additively Manufactured Dogbone Geometries.
Clemson University TigerPrints All Theses Theses 52017 Comparison of Asbuilt FEA Simulations and Experimental Results for Additively Manufactured Dogbone Geometries. Prathamesh Baikerikar Clemson University,
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationPLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES
PLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES Cimini Jr., Carlos A., and Tsai, Stephen W. 2 Department of Mechanical Engineering, Federal University of Minas Gerais Av. Antônio Carlos, 6627
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationEXPERIMENTAL STUDY ON YOUNG S MODULUS E OF A POLYMER COMPOSITE REINFORCED BY NANO TITANIUM DIOXIDE PARTICLES
Vietnam Journal of Mechanics, VAST, Vol. 34, No. (202), pp. 9 25 EXPERIMENTAL STUDY ON YOUNG S MODULUS E OF A POLYMER COMPOSITE REINFORCED BY NANO TITANIUM DIOXIDE PARTICLES Nguyen Dinh Duc, Dinh Khac
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationS HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD
S HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD By Jen Y. Liu 1 and Lester H. Floeter 2 ABSTRACT: In this study, the writers used Tsai and Wu s tensor polynomial theory to rederive a formula originally
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationTensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites
Tensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites Journal of Reinforced Plastics and Composites, Vol. 9 (March, 1990) pp. 127133 W. H. PROSSER NASA Langley Research Center
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationCentrifuge Shaking Table Tests and FEM Analyses of RC Pile Foundation and Underground Structure
Centrifuge Shaking Table s and FEM Analyses of RC Pile Foundation and Underground Structure Kenji Yonezawa Obayashi Corporation, Tokyo, Japan. Takuya Anabuki Obayashi Corporation, Tokyo, Japan. Shunichi
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationLinearTime Thermal Simulation of AsManufactured FDM Components
LinearTime Thermal Simulation of AsManufactured FDM Components Yaqi Zhang and Vadim Shapiro Spatial Automation Laboratory University of Wisconsin  Madison Madison, Wisconsin 53706 August 2017 Abstract
More informationMechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method
, pp.6782 http://dx.doi.org/1.14257/ijast.215.78.6 Mechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method P. Prasanthi
More informationUsing MATLAB to Compute Heat Transfer in Free Form Extrusion
22 Using MATLAB to Compute Heat Transfer in Free Form Extrusion Sidonie Costa, Fernando Duarte and José A. Covas University of Minho Portugal 1. Introduction Rapid Prototyping (RP) is a group of techniques
More informationRegular, low density cellular structures  rapid prototyping, numerical simulation, mechanical testing
Mat. Res. Soc. Symp. Proc. Vol. 823 2004 Materials Research Society W8.8.1 Regular, low density cellular structures  rapid prototyping, numerical simulation, mechanical testing J. Stampfl 1, M.M. Seyr
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationSTRESSLIMITING TEST STRUCTURES FOR RAPID LOWCOST STRENGTH ASSESSMENT
STRESSLIMITING TEST STRUCTURES FOR RAPID LOWCOST STRENGTH ASSESSMENT A. Katz, J. Nussbaum, N. B. Crane, C. P. Lusk Mechanical Engineering Department, University of South Florida, Tampa, Florida, 33620
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM BEHAVIOR UNDER THE EFFECT OF EXTERNAL SOLICITATIONS
Third International Conference on Energy, Materials, Applied Energetics and Pollution. ICEMAEP016, October 3031, 016, Constantine,Algeria. ANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationProceedings of the ASME th International Conference on Ocean, Offshore and Arctic Engineering OMAE2016 June 1924, 2016, Busan, South Korea
Proceedings of the ASME 26 35th International Conference on Ocean, Offshore and Arctic Engineering OMAE26 June 924, 26, Busan, South Korea OMAE2654554 LOCAL STRAIN AND STRESS CALCULATION METHODS OF IRREGULAR
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationTOWARD VIRTUAL CERAMIC COMPOSITES
TOWARD VIRTUAL CERAMIC COMPOSITES M. Genet 1, P. Ladevèze 12, G. Lubineau 1 1 LMTCachan (ENSCachan, CNRS, Paris 6 University, UniverSud Paris PRES) 61 avenue du Président Wilson 94235 Cachan CEDEX {genet,
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationDIGIMAT for NANOCOMPOSITES
DIGIMAT for NANOCOMPOSITES Document Version 2.0.1, February 2010 info@exstream.com www.exstream.com Materials: Engineering Plastics, Reinforced Plastics, Mineral and Clay fillers. exstream Technology:
More informationNONLINEAR ELASTIC CONSTITUTIVE RELATIONS FOR CELLULOSIC MATERIALS
In: Perkins, R.W., ed. Mechanics of cellulosic and polymeric materials: Proceedings, 3d Joint ASCE/ASME Mechanics conference; 1989 July 912; San Diego, New York: The American Society of Mechanical Engineers;
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationSimulation Analysis of Microchannel Deformation during LTCC Warm Water Isostatic Pressing Process Lang Ping, Zhaohua Wu*
International Conference on Information Sciences, Machinery, Materials and Energy (ICISMME 2015) Simulation Analysis of Microchannel Deformation during LTCC Warm Water Isostatic Pressing Process Lang Ping,
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationModeling and Simulation to Materials Development for Rapid Prototyping Process
Modeling and Simulation to Materials Development for Rapid Prototyping Process Jardini A.L., M.C.B. Costa, R.A. Rezende, Andrade S.R., Maciel Filho R. Laboratory of Optimization, Project and Advanced Control
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationFinite element simulation of residual stresses in laser heating
IAS200866546ST Finite element simulation of residual stresses in laser heating G. H. Farrahi 1, M. Sistaninia 2, H. Moeinoddini 3 1,2School of Mechanical Engineering, Sharif University of Technology,
More informationCOURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.)
Narvik University College (Høgskolen i Narvik) EXAMINATION TASK COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.) CLASS: Master students in Engineering Design
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationSimulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias
As originally published in the IPC APEX EXPO Conference Proceedings. Simulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias Yan Ning, Michael H. Azarian, and Michael
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationFormulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading
Formulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading Debaroti Ghosh & Mahbuba Begum Dept of Civil Engineering, Bangladesh University of Engineering
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationIMPACT OF LAMINATE DIRECTIONS ON IN PLANE SHEAR STIFFNESS OF CROSS LAMINATED TIMBER
IMPACT OF LAMINATE DIRECTIONS ON IN PLANE SHEAR STIFFNESS OF CROSS LAMINATED TIMBER Turesson, J. 1 & Ekevad, M. 2 ABSTRACT Twentythree finite element models of crosslaminated timber (CLT) with different
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More information